Create Presentation
Download Presentation

Download Presentation
## Density, Volume, and Packing: Part 2 Thursday, September 4, 2008

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -

**Density, Volume, and Packing: Part 2Thursday, September 4,**2008 Steve Feller Coe College Physics Department Lecture 3 of Glass Properties Course**Some Definitions**• x = molar fraction of alkali or alkaline-earth oxide (or any modifying oxide) • 1-x = molar fraction of glass former • R = x/(1-x) This is the compositional parameter of choice in developing structural models for borates. • J = x/(1-x) for silicates and germanates**Short Ranges B and Si Structures**Short-range borate units, Short-range silicate units,**Method of Least Squares**• Take (ρmod – ρexp)2 for each data point • Add up all terms • Vary volumes until a least sum is found. • Volumes include empty space. • ρmod = M/(fiVi)**Example: Li-Silicates**VQ4 = 1.00 VQ3 = 1.17 VQ2 = 1.41 VQ1 = 1.69 VQ0 = 1.95 VQ4(J = 0) defined to be 1. The J = 0 glass is silicon dioxide with density of 2.205 g/cc**Borate Structural Model**• R < 0.5 • F1 = 1-R, F2 = R • 0.5 <R <1.0 • F1 = 1-R, F2 = -(1/3)R +2/3, F3 = +(4/3)R -2/3 • 1.0 <R < 2.0 • F2 = -(1/3)R +2/3, F3 = -(2/3)R +4/3 , F4 = R-1**Another Example: Li-Borates**• V1 = 0.98 • V2 = 0.91 • V3 = 1.37 • V4 = 1.66 • V5 = 1.95 • V1(R = 0) is defined to be 1. • The R = 0 glass is boron oxide with density of 1.823 g/cc**Li and Ca Silicates**Li Ca VQ4 = 1.00 VQ4 = 1.00 VQ3 = 1.17 VQ3 = 1.20 VQ2 = 1.41 VQ2 = 1.46 VQ4(J = 0) defined to be 1. The J = 0 glass is silicon dioxide with density of 2.205 g/cc**Densities of Barium Borate Glasses**• R = x/(1-x) Density (g/cc) • 0·0 1·82 • 0·2 2·68 • 0·2 2·66 • 0·4 3·35 • 0·4 3·29 • 0·6 3·71 • 0·6 3·68 • 0·8 3·95 • 0·8 3·90 • 0·9 4·09 • 1·2 4·22 • 1·3 4·31 • 1·5 4·40 • 1·7 4·50 • 2·0 4·53 Use these data and the borate model to find the four borate volumes. Note this model might not yield exactly the volumes given before.**Volumes and packing fractions of borate short-range order**groups. The volumes are reported relative to the volume of the BO1.5 unit in B2O3 glass. Packing fractions were determined from the density derived volumes and Shannon radii[i],[ii]. • System Unit Least Squares Volumes Packing Fraction • Li f1 0.98 0.34 • f2 0.94 0.65 • f3 1.28 0.39 • f4 1.61 0.41 • Na f1 0.95 0.35 • f2 1.24 0.62 • f3 1.58 0.41 • f4 2.12 0.46 • K f1 0.95 0.35 • f2 1.66 0.69 • f3 1.99 0.52 • f4 2.95 0.59 • Rb f1 0.98 0.34 • f2 1.92 0.67 • f3 2.27 0.52 • f4 3.41 0.59 • Cs f1 0.97 0.34 • f2 2.28 0.67 • f3 2.62 0.54 • f4 4.13 0.61 • [i] Barsoum, Michael, Fundamentals of Ceramics (McGraw-Hill: Columbus OH,1997), 85-89. • [ii] R.D. Shannon, Acta. Crystallogr., A32 (1976), 751.**System Unit Least Squares Volumes Packing Fraction**• Mg f1 0.98 0.34 • f2 0.95 0.63 • f3 1.26 0.39 • f4 1.46 0.44 • Ca f1 0.98 0.34 • f2 0.95 0.71 • f3 1.28 0.44 • f4 1.66 0.48 • Sr f1 0.94 0.36 • f2 1.08 0.68 • f3 1.41 0.45 • f4 1.92 0.48 • Ba f1 0.97 0.35 • f2 1.13 0.73 • f3 1.55 0.47 • f4 2.16 0.51**Volumes and packing fractions of silicates short-range**order groups. The volumes are reported relative to the volume of the Q4 unit in SiO2 glass. Packing fractions were determined from the density derived volumes and Shannon radii4,23. • System Unit Least Squares Volumes Packing Fraction • Li Q4 1.00 0.33 • Q3 1.17 0.38 • Q2 1.41 0.41 • Q1 1.67 0.42 • Q0 1.92 0.43 • Na Q4 1.00 0.33 • Q3 1.34 0.42 • Q2 1.74 0.46 • Q1 2.17 0.48 • Q0 2.63 0.49 • K Q4 0.99 0.33 • Q3 1.58 0.52 • Q2 2.27 0.58 • Q1 2.97 0.61 • Rb Q4 1.00 0.33 • Q3 1.72 0.53 • Q2 2.63 0.57 • Q1 3.53 0.59 • Cs Q4 0.98 0.33 • Q3 1.96 0.56 • Q2 2.90 0.64 • Q1 4.25 0.62**Alkali Thioborates**• Data from Prof. Steve Martin • x M2S.(1-x)B2S3 glasses • Unusual F2 behavior**Volumes and packing fractions of thioborate short-range**order groups. The volumes are reported relative to the volume of the BS1.5 unit in B2S3 glass. • System Unit Least Squares Volumes Corresponding Oxide Volume • (compared with volume of BO1.5 unit in B2O3 glass.) • __________________________ • Na f1 1.00 0.95 • f2 1.37 1.24 • f3 1.51 1.58 • f5 2.95 2.66* • K f1 1.00 0.95 • f2 1.65 1.66 • f3 1.78 1.99 • f5 3.53 3.91* • Rb f1 1.00 0.98 • f2 1.79 1.92 • f3 1.97 2.27 • f5 3.90 4.55* • Cs f1 1.00 0.97 • f2 1.83 2.28 • f3 2.14 2.62 • f5 4.46 5.64* • *extrapolated**Molar Volume**• Molar Volume = Molar Mass/density It is the volume per mole glass. It eliminates mass from the density and uses equal number of particles for comparison purposes.**Borate Glasses**Kodama Data**Problem:**• Calculate the molar volumes of the barium borates given before. You will need atomic masses. Also, remember that the data are given in terms of R and there are R+1 moles of glassy materials. You could also use x to do the calculation.**Li-Vanadate (yellow) Molar Volumes campared with**Li-Phosphates (black)**Rb -purple squares**Cs -yellow triangles**K- open circles**Rb -purple squares Cs -yellow triangles**Differential Changes in Unit Volumes**• To begin the calculation, we define the glass density in terms of its dimensionless mass relative to pure borate glass (R=0), m′(R), and its dimensionless volume relative to pure borate glass, v′(R):**Solve for v1 and v2 simultaneously and assign it to R = (R1**+R2)/2 • This is accurate if R1 and R2 are close to each other; in Kodama’s data this condition is met.**The Volume per Mole Glass Former**• Volume per mole glass former = Mass (JM2O.SiO2)/density It is the volume per mole glass former and R moles of modifier.**The Volume per Mole Glass Former**• Why is there a trend linear? • JM2O.SiO2 (1-2J)Q4 +2JQ3J<0.5 • So slope of volume curve is the additional volume needed to form Q3 at the expense of Q4. This is proportional to J.**Sodium Borogermanates Volumes per Mol B2O3 Compared to**Sodium Borosilicates**Problem**• For the barium borate data provided earlier plot the volume per mol boron oxide as a function of R. • How do you interpret the result? Lecture 2 ends here**Packing in Glass**• We will now examine the packing fractions obtained in glasses. This will provide a dimensionless parameter that displays some universal trends. • We will need a good knowledge of the ionic radii. This will be provided next.